DOI: 10.17188/1722175
title: Materials Data on Li15V6(P8O29)2 by Materials Project

description: Li15V6(P8O29)2 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are fifteen inequivalent Li sites. In the first Li site, Li is bonded in a distorted see-saw-like geometry to four O atoms. There are a spread of Li–O bond distances ranging from 1.98–2.10 Å. In the second Li site, Li is bonded to four O atoms to form distorted LiO4 tetrahedra that share corners with two LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.93–2.31 Å. In the third Li site, Li is bonded to four O atoms to form distorted LiO4 tetrahedra that share corners with two LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.95–2.21 Å. In the fourth Li site, Li is bonded to four O atoms to form LiO4 tetrahedra that share corners with three VO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 69–71°. There are a spread of Li–O bond distances ranging from 1.86–2.21 Å. In the fifth Li site, Li is bonded in a distorted see-saw-like geometry to four O atoms. There are a spread of Li–O bond distances ranging from 2.02–2.08 Å. In the sixth Li site, Li is bonded to four O atoms to form distorted LiO4 tetrahedra that share corners with four PO4 tetrahedra and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.98–2.08 Å. In the seventh Li site, Li is bonded to four O atoms to form distorted LiO4 tetrahedra that share corners with two LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.94–2.20 Å. In the eighth Li site, Li is bonded to four O atoms to form distorted LiO4 tetrahedra that share corners with two LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.94–2.13 Å. In the ninth Li site, Li is bonded in a 4-coordinate geometry to four O atoms. There are a spread of Li–O bond distances ranging from 1.98–2.13 Å. In the tenth Li site, Li is bonded in a distorted see-saw-like geometry to four O atoms. There are a spread of Li–O bond distances ranging from 2.00–2.08 Å. In the eleventh Li site, Li is bonded to four O atoms to form LiO4 tetrahedra that share corners with three VO6 octahedra and corners with four PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 65–66°. There are a spread of Li–O bond distances ranging from 1.88–2.16 Å. In the twelfth Li site, Li is bonded to four O atoms to form distorted LiO4 tetrahedra that share corners with two LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.97–2.17 Å. In the thirteenth Li site, Li is bonded to four O atoms to form distorted LiO4 tetrahedra that share corners with two LiO4 tetrahedra, corners with four PO4 tetrahedra, and an edgeedge with one VO6 octahedra. There are a spread of Li–O bond distances ranging from 1.95–2.23 Å. In the fourteenth Li site, Li is bonded in a distorted see-saw-like geometry to four O atoms. There are a spread of Li–O bond distances ranging from 1.97–2.12 Å. In the fifteenth Li site, Li is bonded in a 6-coordinate geometry to six O atoms. There are a spread of Li–O bond distances ranging from 2.26–2.46 Å. There are six inequivalent V sites. In the first V site, V is bonded to six O atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.88–2.00 Å. In the second V site, V is bonded to six O atoms to form VO6 octahedra that share corners with two LiO4 tetrahedra, corners with six PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 2.02–2.06 Å. In the third V site, V is bonded to six O atoms to form VO6 octahedra that share corners with two LiO4 tetrahedra, corners with six PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.86–2.02 Å. In the fourth V site, V is bonded to six O atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and edges with two LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.85–2.02 Å. In the fifth V site, V is bonded to six O atoms to form VO6 octahedra that share corners with six PO4 tetrahedra and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 1.96–2.07 Å. In the sixth V site, V is bonded to six O atoms to form VO6 octahedra that share corners with two LiO4 tetrahedra, corners with six PO4 tetrahedra, and an edgeedge with one LiO4 tetrahedra. There are a spread of V–O bond distances ranging from 2.00–2.07 Å. There are sixteen inequivalent P sites. In the first P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 49°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the second P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with three LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 38–48°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the third P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with three LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 43–47°. There are a spread of P–O bond distances ranging from 1.51–1.63 Å. In the fourth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 39–40°. There are a spread of P–O bond distances ranging from 1.52–1.58 Å. In the fifth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and corners with three LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–35°. There are a spread of P–O bond distances ranging from 1.49–1.62 Å. In the sixth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 48–49°. There are a spread of P–O bond distances ranging from 1.53–1.61 Å. In the seventh P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with four LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 49–50°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the eighth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with two LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 46–49°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the ninth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 41–46°. There are a spread of P–O bond distances ranging from 1.52–1.61 Å. In the tenth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with three LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 41–47°. There are a spread of P–O bond distances ranging from 1.50–1.61 Å. In the eleventh P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedra tilt angles range from 40–47°. There is three shorter (1.53 Å) and one longer (1.62 Å) P–O bond length. In the twelfth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with three VO6 octahedra and corners with four LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 36–38°. There are a spread of P–O bond distances ranging from 1.51–1.58 Å. In the thirteenth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with three VO6 octahedra. The corner-sharing octahedra tilt angles range from 33–38°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the fourteenth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with four LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 49–51°. There are a spread of P–O bond distances ranging from 1.51–1.62 Å. In the fifteenth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one PO4 tetrahedra, and corners with four LiO4 tetrahedra. The corner-sharing octahedra tilt angles range from 47–50°. There are a spread of P–O bond distances ranging from 1.50–1.62 Å. In the sixteenth P site, P is bonded to four O atoms to form PO4 tetrahedra that share corners with two VO6 octahedra, a cornercorner with one LiO4 tetrahedra, and a cornercorner with one PO4 tetrahedra. The corner-sharing octahedral tilt angles are 44°. There are a spread of P–O bond distances ranging from 1.51–1.61 Å. There are fifty-eight inequivalent O sites. In the first O site, O is bonded in a trigonal planar geometry to two Li and one P atom. In the second O site, O is bonded in a distorted trigonal planar geometry to one Li, one V, and one P atom. In the third O site, O is bonded to three Li and one P atom to form distorted corner-sharing OLi3P trigonal pyramids. In the fourth O site, O is bonded in a distorted trigonal planar geometry to one Li, one V, and one P atom. In the fifth O site, O is bonded in a distorted trigonal planar geometry to one Li, one V, and one P atom. In the sixth O site, O is bonded in a distorted trigonal planar geometry to one Li, one V, and one P atom. In the seventh O site, O is bonded in a distorted bent 150 degrees geometry to one V and one P atom. In the eighth O site, O is bonded to three Li and one P atom to form distorted corner-sharing OLi3P trigonal pyramids. In the ninth O site, O is bonded in a distorted trigonal planar geometry to one Li, one V, and one P atom. In the tenth O site, O is bonded in a distorted T-shaped geometry to one Li, one V, and one P atom. In the eleventh O site, O is bonded in a bent 150 degrees geometry to one V and one P atom. In the twelfth O site, O is bonded in a 3-coordinate geometry to one Li, one V, and one P atom. In the thirteenth O site, O is bonded in a linear geometry to one Li and one P atom. In the fourteenth O site, O is bonded in a single-bond geometry to one P atom. In the fifteenth O site, O is bonded in a distorted trigonal non-coplanar geometry to one Li, one V, and one P atom. In the sixteenth O site, O is bonded in a distorted trigonal planar geometry to one Li, one V, and one P atom. In the seventeenth O site, O is bonded in a distorted trigonal non-coplanar geometry to one Li, one V, and one P atom. In the eighteenth O site, O is bonded in a trigonal planar geometry to one Li, one V, and one P atom. In the nineteenth O site, O is bonded in a bent 150 degrees geometry to two P atoms.